Fabrication and low-temperature transport properties of selectively grown
dual-gated single-electron transistors
J. Motohisa,a)F. Nakajima, and T. Fukui
Research Center for Integrated Quantum Electronics, Hokkaido University, North 13 West 8, Sapporo 060-8628, Japan
W. G. van der Wiel, J. M. Elzerman, and S. De Franceschi, and L. P. Kouwenhoven Department of Applied Physics and DIMES, Delft University of Technology, P. O. Box 5046, 2600 GA Delft, The Netherlands
共Received 14 January 2002; accepted for publicztion 25 February 2002兲
We report on the fabrication of a dual-gated single-electron transistor共SET兲 based on a quantum dot 共QD兲 formed by selective area growth of metalorganic vapor-phase epitaxy, and its low-temperature transport properties. We observe clear Coulomb oscillations in a SET fabricated in combination with direct growth of nanostructures and lithographically defined metal gates. The magnetic field dependence of the Coulomb oscillations as well as the Coulomb diamonds suggest strong carrier confinement in our QD. © 2002 American Institute of Physics. 关DOI: 10.1063/1.1470246兴
Single-electron transport through semiconductor quan-tum dots共QDs兲 has recently attracted considerable attention. From the application point of view, single-electron devices utilizing Coulomb blockade effects have the potential to re-alize circuits with high-density integration and low power consumption.1 From the physics point of view, the three-dimensional confinement in a QD gives rise to a discrete energy spectrum in analogy to atoms. The shell structure can be detected by single-electron transport.2Furthermore, when the QD has a net spin, it can be considered as a localized magnetic impurity with tunable parameters, offering a play-ground for tunable Kondo physics.3Realization of very small QDs is required for possible operation at high temperatures. We have reported before on the fabrication of single-electron devices and circuits by using selective area metalor-ganic vapor-phase epitaxy 共SA-MOVPE兲 on partially masked substrates.4 – 6 SA-MOVPE technology allows us to fabricate various kinds of semiconductor quantum nanostruc-tures and their dense arrays only with one-step growth by using appropriate mask designing of the substrate. Therefore, it is possible to realize integrated circuits based on nano-structures and single-electron devices.5In particular, we have recently reported on quantum dot arrays and dot-wire coupled structures by utilizing a zig-zag mask pattern.7 We also have proposed single-electron transistors共SETs兲 having much smaller QDs and stronger lateral confinement as com-pared to our conventional structures, and SET operation has partially been demonstrated.
So far, our study of the transport properties of SETs fabricated by SA-MOVPE was limited to a narrow tempera-ture region and Coulomb oscillations were observed only in a limited range of gate and source-drain voltages. In this letter, we extend our investigation to low temperature mea-surements. The implementation of dual-gated structures en-hance the tunability of the potential of the QD and tunneling barriers. We have demonstrated clear Coulomb oscillations
in a SET fabricated in combination with crystal growth and dual gates defined by lithographic techniques. Our devices have shown the possibility to explore single-electron trans-port and the Kondo effect, owing to strong confinement.
The secondary electron microscopy共SEM兲 image of the present QD device is shown in Fig. 1共a兲. For its fabrication, we first prepare a masked substrate of Fig. 1共b兲. Starting with a SiON-coated GaAs 共001兲 substrate, SiON in the zig-zag shaped area is partly removed by electron-beam lithography wet chemical etching. The edges of the opening are either along the 关110兴 or 关010兴 directions. Next, a n-AlGaAs/GaAs/AlGaAs selectively doped double hetero-structure is grown by MOVPE on an opening area where the 共001兲 GaAs surface is exposed. Because of the evolution of
兵111其B and兵110其 facet sidewalls during the growth, we have a width modulated channel of the two-dimensional electron gas共2DEG兲 in the GaAs layer following the mask pattern, as shown in Fig. 1共c兲. As a result, a small, diamond-shaped 2DEG region is formed in between two constrictions. Details of the growth process are reported elsewhere.7Then, we de-fine two gates, a top gate and a side gate, near this region, as shown in the SEM image. The QD is formed between the
a兲Author to whom correspondence should be addressed; electronic mail:
FIG. 1.共a兲 SEM image of the device. Schematic illustration of 共b兲 the mask pattern and共c兲 layer structure.
APPLIED PHYSICS LETTERS VOLUME 80, NUMBER 15 15 APRIL 2002
0003-6951/2002/80(15)/2797/3/$19.00 © 2002 American Institute of Physics
two constrictions when a negative top gate voltage is ap-plied. The big reservoirs on both sides of the QD correspond to the source and drain contacts.
In this device, the top gate changes both the electrostatic potential of the QD and the tunneling barrier characteristics.7 On the other hand, the side gate mainly effects the electro-static potential of the dot, although some effect on the barri-ers and confinement is unavoidable. Thus, the present dual-gated structure allows one to control the electrostatic potential of the QD nearly independently of the tunneling resistance and the dot shape. Hence, we can investigate single-electron transport in the case of weak and strong cou-pling of the QD to its leads. Since the channel lays about 50 nm beneath the surface, we estimate the geometrical size of the dot to be 320 nm, which is slightly larger than the devices reported previously.7 The QD becomes effectively smaller by the application of a negative top gate voltage. The electron concentration and mobility of 2DEG formed on the unmasked reference substrate is 8.5⫻1011cm⫺2 and 6.6 ⫻104 cm2/V s, respectively, at 77 K. The sample is mea-sured in a dilution refrigerator with a base temperature of 15 mK. We measure the source–drain conductance, G, of the device with a constant dc bias of 10V, or the differ-ential conductance dIDS/dVDS using a lock-in technique with an ac bias of 5V superimposed on the dc bias, VDS. Without applying a negative top gate voltage, VTG, the conductance through the QD hardly changes when sweeping the side gate voltage, VSG. However, by applying a voltage more negative than about ⫺250 mV to VTG, the conduc-tance shows Coulomb oscillations as a function of VSG. Fig-ure 2共a兲 shows typical Coulomb oscillations for different top gate voltages. At the same time, the peak of the oscillations shifts to more negative side gate values when VTG is made more positive. Similar Coulomb oscillations for VSG and their shift with respect to VTG are observed for ⫺265 mV ⬍VTG⬍⫺285 mV, as shown in Fig. 2共b兲. For these top gate voltages, the valley conductance as well as the Coulomb peaks seem to be enhanced, as the tunneling resistance of the barrier is reduced as compared to the case of more negative VTG. These results clearly indicate that a QD is formed in our device by applying a sufficiently negative voltage to the top gate. We note that, in Fig. 2共b兲, a plateau-like structure is observed as indicated by the arrow. We will discuss its origin later. We also note that the peak height also changes with VTGin a nonmonotonic manner. We think that by changing VTG, different wave functions may be involved in transport, resulting in a different tunnel probability.
Figure 3 shows a gray-scale plot of the differential con-ductance, dIDS/dVDS, for VTG⫽⫺299 mV 关thicker trace in Fig. 2共a兲兴. We observe clear Coulomb diamonds. As one can see in Fig. 3, the Coulomb gap UCstrongly depends on the side gate voltage VSG. The maximum and minimum values for UC are 3.30 mV and 1.34 mV, respectively. One of the possible explanations for such a dependence would be the change of the effective dot size by the side gate bias. This would partly explain the results, because the alpha factor8 (␣⫽CG/Cdot, where CG the capacitance between dot and the side gate, Cdotthe total capacitance of the dot兲 increases monotonically when VSGis decreased and CGwould be more sensitive to Cdot for VSG. However, the Coulomb gap does
not show monotonic change for VSG. The second possibility would be the dependence of the addition energy on the num-ber N of electrons in the QD. This can happen, for example, when the QD has a shell structure similar to real atoms共 or artificial atoms兲.2We will come back to this point later.
We also measure the evolution of the Coulomb oscilla-tions with magnetic field. The results are shown in Fig. 4 in a gray-scale plot of conductance, G, as a function of mag-netic field B, and side gate voltage VSG. Here, VTGis fixed at⫺299 mV, and the magnetic field is applied normal to the surface. Although the overall behavior is somewhat compli-cated, the Coulomb peaks show a parabolic shift for 0⬍B ⬍2 T, particularly for the peaks observed at more negative VSG. In addition, we also can see some kinks in the peak shift, which is probably due to the crossing of ground states. In some ranges of magnetic field and side gate voltage, the FIG. 2. Linear conductance of the device measured at base temperature (⬃15 mK), for fixed top gate voltage, VTG. VTG is varied 共a兲 from
⫺305 mV 共top兲 to ⫺285 mV 共bottom兲, and 共b兲 from ⫺285 mV 共top兲 to ⫺265 mV 共bottom兲. The step size for VTGis 1 mV for each figure.
FIG. 3. Gray-scale plot of the differential conductance dISD/VSD, plotted as
a function of both VSDand VSG. The top gate voltage is⫺299 mV. For
VSG⬍0.7 V, the contrast is enhanced by factor of 5.
2798 Appl. Phys. Lett., Vol. 80, No. 15, 15 April 2002 Motohisaet al.
peaks are suppressed considerably. On the other hand, peaks reappear around 1.8⬍B⬍2.8 T, for VSG⬃⫺1.25 V. Such behavior of the peaks could suggest that there is an overlap of the wave functions in the QD which leads to changes by the magnetic field and gate voltages in a rather complicated fashion. However, these characteristics are not clearly under-stood yet.
From the results of Figs. 3 and 4, we estimate the peak shift by the magnetic field at 2 T is order of 0.12 meV. This small shift of the Coulomb peaks for 0⬍B⬍2 T strongly suggests that the carrier confinement in our QD is strong and the number N of electrons in a QD is very small. The simi-larity of the magnetic field dependence between our present results and the results of Tarucha et al.2also forms evidence for strong confinement of a small number of electrons and atomic-like properties in our QD. On the other hand, the level separation estimated from the excited state spectrum, is very small (0.18– 0.30 meV) and does not imply strong quantum confinement. It is difficult to obtain an estimate for N derived from the dot diameter, d 共estimated from the maximum charging energy兲, and the electron density.
Now, we would like to discuss the origin of the plateau-like structure indicated by the arrow in Fig. 2共b兲. We think this broad peak originates from the Kondo effect, which is observed when the QD has a net spin 共usually, S⫽ 1/2兲.3 Although we have not measured temperature dependence, systematic measurements,10such as differential conductance, dIDS/dVDSwhere we have observed a characteristic peak at VDS⫽0, strongly suggests the existence of the Kondo effects close to the unitary limit.11Furthermore, our study on higher magnetic field (⬃4.6 T) clearly shows the existence of the Kondo effect in the similar top gate voltage conditions. A detailed study of the Kondo effect at high magnetic field will be presented elsewhere.12
Finally, we describe some of the technological impact of our present device structures. First of all, direct formation methods of nanostructures utilizing epitaxial growth are very effective to realize structures or devices with very small high-density QDs, which we showed in our previous papers. Dilger et al. also have reported low-temperature 共down to 22 mK兲 Coulomb oscillations in a QD device formed by di-rect molecular-beam epitaxial growth on patterned GaAs substrates.9In these devices, the size of the QDs is estimated to be about or less than 150 nm. Secondly, the dual-gated structure enhances the tuning range to observe Coulomb blockade in such epitaxially grown structures. In our previ-ous devices, the gate bias conditions to observe Coulomb oscillations are very limited and are very close to their threshold voltage. In the case of the device of Dilger et al., in which an in-plane gate fabricated during the growth is used to tune the electrostatic potential of the QD, a gradual in-crease of the valley conductance of the Coulomb oscillations is observed. This indicates a dependence of the tunneling resistance between the QD and the leads on the in-plane gate bias. Therefore, the dual-gated structure forms an appealing alternative to enhance the tunability of the QD device. Such gate structure is also advantageous for the application of in-tegrated circuits, such as complementary-type single-electron inverters,13in which control of the peaks of Coulomb oscil-lation is required.
The authors acknowledge Professors H. Hasegawa, H. Akera, M. Eto, and S. Kasai for fruitful discussions. This work is partly financially supported by a Grant-in-Aid for Scientific Research, supported by Ministry of Education, Culture, Sports, Science, and Technology, Japan.
1K. K. Likharev, IEEE Trans. Magn. 23, 1142共1987兲.
2S. Tarucha, D. G. Austing, T. Honda, R. J. van der Hage, and L. P.
Kou-wenhoven, Phys. Rev. Lett. 77, 3613共1996兲.
D. Goldhaber-Gordon, H. Shtrikman, D. Mahalu, D. Abusch-Magder, U. Meirav, and M. A. Kastner, Nature 共London兲 391, 156 共1998兲; S. M. Cronenwett, T. H. Oosterkamp, and L. P. Kouwenhoven, Science 281, 540
共1998兲; J. Schmid, J. Weiss, K. Eberl, and K. von Klitzing, Physica B 256,
K. Kumakura, J. Motohisa, and T. Fukui, Solid-State Electron. 42, 1227
共1998兲; K. Kumakura, J. Motohisa, and T. Fukui, Physica E 共Amsterdam兲
5F. Nakajima, K. Kumakura, J. Motohisa, and T. Fukui, Jpn. J. Appl. Phys.,
Part 1 38, 415共1999兲.
F. Nakajima, J. Motohisa, and T. Fukui, Appl. Surf. Sci. 162, 650共2000兲.
7F. Nakajima, Y. Ogasawara, J. Motohisa, and T. Fukui, J. Appl. Phys. 90,
8J. Weis, R. J. Haug, K. von Klitzing, and K. Ploog, Phys. Rev. Lett. 71,
M. Digler, R. J. Haug, K. Eberl, and K. von Klitzing, Semicond. Sci. Technol. 11, 1493共1996兲.
10J. Motohisa, W. G. van der Wiel, J. M. Elzerman, S. De Franceschi, F.
Nakajima, Y. Ogasawara, T. Fukui, and L. P. Kouwenhoven, Physica E共to be published兲.
11W. G. van der Wiel, S. De Franceschi, T. Fujisawa, J. M. Elzerman, S.
Tarucha, and L. P. Kouwenhoven, Science 289, 2105共2000兲.
12W. G. van der Wiel, S. De Franceschi, J. M. Elzerman, S. Tarucha, L. P.
Kouwenhoven, J. Motohisa, F. Nakajima, and T. Fukui, Phys. Rev. Lett.
共to be published兲.
13J. R. Tucker, J. Appl. Phys. 72, 4399共1992兲.
FIG. 4. Magnetic field dependence of the Coulomb oscillation with respect to the side gate voltage VSG. The top gate voltage is⫺299 mV.
Appl. Phys. Lett., Vol. 80, No. 15, 15 April 2002 Motohisaet al.